Xia et al. – eXPRESS Polymer Letters Vol.6, No.2 (2012) 169–176In this work, a systematic investigation into the mission electron microscope (TEM; JEOL-2100,structures of as-spun nanofiber, the effect of calci- Japan). The electrospinning specimens were sputternation and crystallite growth was conducted for coated with gold before SEM observation, while theunderstanding the formation mechanism of SnO2 SnO2 nanofibers were examined without any fur-hollow nanofibers. In addition, the growth kinetics ther treatment. For TEM observation, the electro-SnO2 nanograin in individual nanofiber was also spun composited nanofibers were directly collectedproposed. on the copper grids for about 30 seconds during electrospinning, while the SnO2 nanofibers were2. Experimental dispersed ultrasonically in ethanol, and then trans-2.1. Preparation of porous hollow SnO2 ferred onto copper grids before TEM observation. nanofibersStannic chloride pentahydrate (SnCl4·5H2O), ethanol 2.3. XRD and TGA analysesand N,N-dimethylformamide (DMF) were pur- The crystal structure analysis was performed on D8chased from Sinopharm Chemical Reagents Co., Advance X-ray diffraction (Bruker AXS, Germany),Shanghai, China. Polyvinylpyrrolidone (PVP, Mw = over the 2! range of 10–80º. Thermogravimetric1300 000 g·mol–1) was supplied by Qi Fuqin Mate- studies were carried out using an SDT 851 thermalrials Technology Co., LTD. Shanghai, China. Trans- analyzer system (Mettler, Germany) at a heatingparent spinning solution was prepared by adding 3 g rate of 10°C/min.of SnCl4·5H2O into 10 wt% PVP in ethanol/DMFsolvent mixture (weight ratio 1:1), and the weight 2.4. Surface area measurementratio of PVP and SnCl4·5H2O was also 1:1, followed The porosity and specific surface areas of the elec-by magnetic stirring at ambient temperature. Subse- trospun fibers were measured by N2 adsorption-quently, the solution was electrospun from the desorption isotherm at 77 K with a Micromeriticsstainless steel needle with an electrostatic voltage NOVA2000e apparatus (Quantachrome, America).of 18 kV, and formed a fibrous mat on a collector ofaluminum foil. The distance between the needle and 3. Results and discussioncollector was 22 cm. The electrospun fibers were 3.1. Structure observationsthen calcinated at 600°C for 3 hrs with a heating Figure 1 demonstrates the morphologies of the elec-rate of 0.5°C/min. trospun nanofibers before and after calcination at 600°C. The as-spun PVP/SnO2 nanofibers have a2.2. Structural observations variable diameter ranged between 50 and 300 nmThe structures of the electrospun nanofibers were and form a self-supporting network, as shown inobserved by a scanning electron microscope (SEM; Figure 1a. The TEM image clearly reveals the core-Hitachi S-4800, Japan) and a high-resolution trans- shell structure with clear boundary of a phase sepa-Figure 1. SEM images of (a) as- spun PVP/SnO2 nanofibers (b) porous hollow SnO2 nanofibers after calcination at 600°C 170
Xia et al. – eXPRESS Polymer Letters Vol.6, No.2 (2012) 169–176 calcination. Based on the TEM observations com- bined TGA/DTGA analysis, the formation process of SnO2 nanofibrous structures can be traced. At the initial stage during electrospinning, the core-shell fibers are fabricated via single capillary electrospin- ning from homogeneous polymer-sol-double sol- vents system due to solvent evaporation and rapid phase separation . Various factors may have strong influences on the morphology of the electro- spun fibers due to the complexity of hydrolysis and condensation reactions during the gelation of sol as well as the process of fiber formation. The hydroly- sis reaction of SnCl4 in water is schematically illus- trated in Figure 3. In this work, excessive ethanol was applied to prepare Sn precursor but insufficient H2O was used to make it partially hydrolyzed. Thus, the polymerization and polycondensation reactionsFigure 2. TEM images of as-spun PVP/SnO2 nanofibers at room temperature of tin dioxide could be limited to a very low level. Furthermore, a kind of more volatile solvent ethanolration between PVP and Sn precursor, as presented evaporates rapidly at the edge of the fiber and ain Figure 2. contrary concentration gradient of ethanol and DMFFigure 1b shows the image of SnO2 nanofibers along the radial direction of the fiber will be formedobtained by the calcination treatment of as-spun during electrospinning. Especially, ethanol, thecore-shell PVP/SnO2 nanofibers. It can be clearly 50% weight ratio of solvents, which was used forseen that these fibers have a tubular structure with preparation tin alkoxide, on the surface of the fibersdense shells, which consist of nanograins of approxi- is too little to form large solvent-rich regions duringmately 17 nm in diameter, as revealed in Figure 1b. the phase separation because of the rapid evapora-Besides SnO2 nanofibers have a relatively uniform tion. The high molecular weight PVP and high con-diameter, the outer diameter of the hollow fibers is centration solution contribute to retain less ethanoldecreased compared to that of the as-spun PVP/ to form porous surface as well. So the smooth andSnO2 fibers shown in Figure 1a. compact surface without any porous structures can be observation by TEM, as revealed in Figure 2. At3.2. Formation of porous hollow SnO2 the same time, Sn precursor in nature has a very nanofibers much higher solubility in ethanol than in PVP .The forming process of hollow SnO2 nanofibers So, it would diffuse from the surface to the core ofexperiences 5 stages during electrospinning and the fiber. As a result, Sn precursor tends to congre-Figure 3. Schematic illustration of the hydrolytic–polymeric reaction of SnCl4·5H2O. Tin, blue; oxygen, red; carbon, pur- ple; hydrogen, white; chlorine, brown. 171
Xia et al. – eXPRESS Polymer Letters Vol.6, No.2 (2012) 169–176 gate at the center of the fiber by the driving force of the concentration gradient of ethanol, resulting in a clear core/shell structure. At the second stage, the first weight loss stage which coincides with the decomposition of PVP chain at the temperature around 280 to 330ºC occurs , as shown in Figure 4. The core-shell nanofibers still exist though the diameter of fiber decreases and the boundaries between core and shell are blurred, as indicated in Figure 5a. Eventually, the core-shell structure disappears after the second endothermicFigure 4. TGA-DTGA graph of thermal decomposition of peak from 350–480ºC (Figure 4) due to the almost electrospun PVP/SnO2 composite nanofibers complete decomposition of PVP, in which the processFigure 5. TEM images of PVP/SnO2 nanofibers (a) calcined at 300ºC, (b) calcined at 400ºC, (c) calcined at 500ºC, (d) cal- cined at 600ºC 172
Xia et al. – eXPRESS Polymer Letters Vol.6, No.2 (2012) 169–176enters the third stage. At this stage, the Sn precursor outward transport of fast-moving Sn precursor mol-on the surface region of the electrospun nanofibers ecules (short as Ja in Figure 6) move through theis exposed to air, leading to the decomposition and oxide layer and a balancing inward flow of vacan-oxidation of the precursor and resulted in the for- cies traverse to the vicinity of the Sn precursors andmation of SnO2. Thus some small SnO2 particles are Sn precursors/SnO2 mixture interface (a/ab inter-presented on the surface whereas most Sn precursor face) and vacancies assisted exchange of materialinside the fibers remains unreacted due to the absence depends on the way of bulk inter-diffusion, as illus-of oxygen, leading to solid fiber structure with par- trated in Figure 6b. Then, the voids are just liketicles on surface, as illustrated in Figure 5b. When sinks to transfer the inward flux of vacancies (Jc =the forming process enters the fourth stage which is Ja – Jb) and the voids coalesce into bigger ones soa complicated transformation process including as to touch the compound layer ab. Such new bridgesgrain formation, grain growth and grain reorganiza- are established as fast transport paths for the remain-tion. Figure 5c may be one of morphological situa- ing Sn precursors (Figure 6c). At this stage, the sur-tion during this process. Nanograins are the main face diffusion takes over the dominant materialcomponents to build solid body though the fibers transport process because the porous surface ownsappear to be irregular. Finally, the hollow SnO2 much lower apparent activation energy than thosenanofibers are formed with porous nanograins on of bulk diffusion . Sn precursors can be quicklythe shell, as shown in Figure 5d oxidized at the surface of ab layer and redistributeAccording to TEM observations of the hollow SnO2 themselves via fast surface diffusion, while the abnanofibers formation, it is clearly revealed that PVP layer remains bulk inter-diffusion associated withand Sn precursor are the main constituents of core- Kirkendall effect until the whole Sn precursors turnshell as-spun nanofibers. Then PVP is gradually into SnO2. Therefore, SnO2 stands on the shell anddecomposed during the calcination process. In this vacancies are continuously generated and flowprocess, PVP plays the role of sacrificial template, inward to build a hollow core, as shown in Fig-which is the key effect to maintain fibrous struc- ure 6d. In all, the fibrous structure is established bytures. The decomposition of PVP, to some extent, PVP template and Kirkendall effect contributions toreduces the final fiber diameters. The key mecha- form hollow structure. Furthermore, surface diffusionnism responsible for the formation of hollow also plays an important role to build hollow fibers.nanofibers is attributed to the interaction between The surface diffusion is also beneficial to the nano-Sn precursor and SnO2 which will be discussed in sized grains growth. In the experiments, the anneal-the next section. ing time (! 4 hrs) obeys the parabolic kinetic equa- tion of grain growth for isothermal annealing as3.3. Analysis of formation mechanism Equation (1):As mentioned above, the main components after the m Dm – D0 = Kt (1)complete decomposition of PVP are some SnO2particles on the surface region and the massive Sn where t is the annealing time, D is the average grainprecursors in the core to form a concentration gradi- size after annealing for time t, D0 is the initial grainent, which lead to a Kirkendall effect . Kirk- size, m is the grain growth exponent, and K is a tem-endall effect is associated with the phenomenon of perature dependent rate constant =1.04·1013 ata considerable amount of compounds moving in or 600ºC .out of a sphere due to the diffusion coupled with The average grain size after 3 hrs calcination isdifferent diffusion rates . When the solid fiber obtained by calculating the size of three intenseconsists of Sn precursor and SnO2 (Figure 6a), the peaks, (110), (101) and (211) of SnO2 from XRDFigure 6. The model for hollow structure formation of SnO2 nanofibers (see text for details) 173
Xia et al. – eXPRESS Polymer Letters Vol.6, No.2 (2012) 169–176patterns. When D0 is neglected, the estimated m defined after calcination at 500 and 600ºC, withoutvalue is 13.2, which is inconsistent with the classi- altering their positions but with high intensitycal grain growth value (m = 2~4) , which means because of better crystallization. All the diffractionthe grain growth of the nanograins observed in the peaks are indexed to the tetragonal rutile SnO2, theindividual nanofibers cannot be primarily ascribed only crystalline phase existing in the obtained nano-by lattice diffusion in a pore controlled scheme. fibers.When the new bridges are established to transportthe mass materials as mentioned above, the connec- 3.4. Surface areastion for lattice diffusion are broken and surface dif- Brunauer–Emmett–Teller (BET) gas sorption meas-fusion will enhance the local voids, meanwhile acts urement reveals the surface area of the hollow SnO2as the driving force for grain growth, leading to fibers. The N2 adsorption–desorption isotherm curveacceleration in the speed of coarse grains by the of the porous SnO2 fibers is shown in Figure 8. Itreduction of the free energy of the system. However, exhibits the characteristic of mesopore structures,the growth kinetics of nanograins in hollow SnO2 especially even owns an adsorption at high P/P0,fibers is complicated and needs further investiga- which was also reported as an aggregation of plate-tion. Heating rate should be studied to control the like particles giving rise to slit-shaped pores .morphology of fibers while using the temperature The porous structure is confirmed by the SEMand duration of calcination as a tool to obtain observations shown in Figure 1b. The average poredesired nanograins on nanofiber surfaces have size in the porous SnO2 fibers is approximatelyalready been reported by Park et al. in Ref . 16.2 nm, and the corresponding BET specific sur-XRD patterns in Figure 7 confirm the formation of face area is about 35.8 m2/g (BJH method).SnO2 fibers. The fibers after calcination at 300ºCshow a broad continuum indicating that the crystal-lization of tin oxide just starts at this temperaturebut not sufficient enough to produce the diffractionpatterns. However, the XRD patterns of the fibersafter calcination at 400ºC show the emergence oftetragonal rutile tin oxide crystals with distinctpeaks due to the decomposition of PVP and oxida-tion of some Sn precursors on the fiber surface. Thediffraction peaks become much sharper and well Figure 8. Nitrogen adsorption/desorption isotherms of the hollow SnO2 nanofibers 4. Conclusions In this work, porous hollow SnO2 nanofibers were successfully prepared by electrospinning technique via a single capillary from PVP/Sn precursors/dual solvents system with calcination treatment. During the electrospinning process, a stringent component matching contributes to core-shell structure which provided advantages for preserving fibrous struc- tures based on sacrificial PVP template. Hollow structures initiated by the Kirkendall effect owing to the concentration gradient of Sn precursors andFigure 7. XRD patterns of SnO2 nanofibres at different SnO2, suggesting that surface diffusion processes temperature 174
Xia et al. – eXPRESS Polymer Letters Vol.6, No.2 (2012) 169–176might be the dominant mass flow mechanism respon-  Xu L., Dong B., Wang Y., Bai X., Liu Q., Song H.:sible for the enlargement of the interior pores after Electrospinning preparation and room temperature gas sensing properties of porous In2O3 nanotubes andinitially formation induced by the Kirkendall effect. nanowires. Sensors and Actuators B: Chemical, 147,This deduction was also confirmed by the calcu- 531–538 (2010).lated grain growth value which was higher than the DOI: 10.1016/j.snb.2010.04.003classical one, which means the grain growth mech-  Soares A. J., Perry R. J.: Modeling and simulation of aanism occurred not only by the lattice diffusion but single tin dioxide nanobelt FET for chemical sensors.also through surface diffusion. This mechanism IEEE Sensors Journal, 10, 235–242 (2010). DOI: 10.1109/JSEN.2009.2032154should also apply to the synthesys of other hollow  Qiu Y., Chen P., Liu M.: Evolution of various por-nanofibers. The technique described here will be phyrin nanostructures via an oil/aqueous medium: Con-extendible to many other materials for fabricating trolled self-assembly, further organization, and supra-such hollow inorganic nanofibers with potential molecular chirality. Journal of the American Chemicalapplications in catalysis, microelectronics, and Society, 132, 9644–9652 (2010).optics. DOI: 10.1021/ja1001967  Park J. Y., Choi S-W., Kim S. S.: A synthesis and sens- ing application of hollow ZnO nanofibers with uni-Acknowledgements form wall thicknesses grown using polymer templates.The research was supported by the specialized Research Nanotechnology, 21, 475601 (2010).Fund for the Doctoral Program of higher education DOI: 10.1088/0957-4484/21/47/475601(No.20090093110004) and National Natural Science Foun-  Chen H., Wang N., Di J., Zhao Y., Song Y., Jiang L.:dation of China (No.51006046 and No.51163014). Nanowire-in-microtube structured core/shell fibers via multifluidic coaxial electrospinning. Langmuir, 26, 11291–11296 (2010).References DOI: 10.1021/la100611f  Song X., Qi Q., Zhang T., Wang C.: A humidity sensor  Cheng Y., Huang W., Zhang Y., Zhu L., Liu Y., Fan X., based on KCl-doped SnO2 nanofibers. Sensors and Cao X.: Preparation of TiO2 hollow nanofibers by Actuators B: Chemical, 138, 368–373 (2009). electrospining combined with sol–gel process. Cryst- DOI: 10.1016/j.snb.2009.02.027 EngComm, 12, 2256–2260 (2010).  Zhang Y., Li J. P., An G. M., He X.: Highly porous DOI: 10.1039/b922564a SnO2 fibers by electrospinning and oxygen plasma  Li L., Yin X., Liu S., Wang Y., Chen L., Wang T.: Elec- etching and its ethanol-sensing properties. Sensors and trospun porous SnO2 nanotubes as high capacity anode Actuators B: Chemical, 144, 43–48 (2010). materials for lithium ion batteries. Electrochemistry DOI: 10.1016/j.snb.2009.10.012 Communications, 12, 1383–1386 (2010).  Zhang Z., Shao C., Li X., Zhang L., Xue H., Wang C., DOI: 10.1016/j.elecom.2010.07.026 Liu Y.: Electrospun nanofibers of ZnO–SnO2 hetero-  Zhang K., Wang X., Yang Y., Wang L., Zhu M., Hsiao junction with high photocatalytic activity. Journal of B., Chu B.: Aligned and molecularly oriented semihol- Physical Chemistry C, 114, 7920–7925 (2010). low ultrafine polymer fiber yarns by a facile method. DOI: 10.1021/jp100262q Journal of Polymer Science Part B: Polymer Physics,  Yang Z., Du G., Feng C., Li S., Chen Z., Zhang P., Guo 48, 1118–1125 (2010). Z., Yu X., Chen G., Huang S., Liu H.: Synthesis of uni- DOI: 10.1002/polb.22003 form polycrystalline tin dioxide nanofibers and elec-  Wang W., Zhou J., Zhang S., Song J., Duan H., Zhou trochemical application in lithium-ion batteries. Elec- M., Gong C., Bao Z., Lu B., Li X., Lan W., Xie E.: A trochimica Acta, 55, 5485–5491 (2010). novel method to fabricate silicananotubes based on DOI: 10.1016/j.electacta.2010.04.045 phase separation effect. Journal of Materials Chem-  Gong S., Liu J., Xia J., Quan L., Liu H., Zhou D.: Gas istry, 20, 9068–9072 (2010). sensing characteristics of SnO2 thin films and analyses DOI: 10.1039/C0JM02120B of sensor response by the gas diffusion theory. Materi-  Loría-Bastarrachea M. I., Herrera-Kao W., Cauich- als Science and Engineering B: Advanced Functional Rodríguez J. V., Cervantes-Uc J. M., Vázquez-Torres Solid-State Materials, 164, 85–90 (2009). H., Ávila-Ortega A.: A TG/FTIR study on the thermal DOI: 10.1016/j.mseb.2009.07.008 degradation of poly(vinyl pyrrolidone). Journal of Thermal Analysis and Calorimetry, 104, 737–742 (2010). DOI: 10.1007/s10973-010-1061-9 175
Xia et al. – eXPRESS Polymer Letters Vol.6, No.2 (2012) 169–176 Yin Y., Rioux R. M., Erdonmez C. K., Hughes S.,  Lai J. K. L., Shek C. H., Lin G. M.: Grain growth Somorjai G. A., Alivisatos A. P.: Formation of hollow kinetics of nanocrystalline SnO2 for long-term isother- nanocrystals through the nanoscale Kirkendall effect. mal annealing. Scripta Materialia, 49, 441–446 (2003). Science, 304, 711–714 (2004). DOI: 10.1016/S1359-6462(03)00296-3 DOI: 10.1126/science.1096566  Park J. Y., Asokan K., Choi S-W., Kim S. S.: Growth Kong J., Tan H. R., Tan S. Y., Li F., Wong S. Y., Li X., kinetics of nanograins in SnO2 fibers and size depend- Lu X.: A generic approach for preparing core–shell ent sensing properties. Sensors and Actuators B: carbon–metal oxide nanofibers: Morphological evolu- Chemical, 152, 254–260 (2011). tion and its mechanism. Chemical Communications, DOI: 10.1016/j.snb.2010.12.017 46, 8773–8775 (2010).  Sing K. S. W., Everett D. H., Haul R. A. W., Moscou DOI: 10.1039/C0CC03006F L., Pierotti R. A., Rouquérol J., Siemieniewska T.: Fan H. J., Knez M., Scholz R., Hesse D., Nielsch K., Reporting physisorption data for gas/solid systems Zacharias M., Gösele U.: Influence of surface diffu- with special reference to the determination of surface sion on the formation of hollow nanostructures induced area and porosity. Pure and Applied Chemistry, 57, by the Kirkendall effect:" The basic concept. Nano Let- 603–619 (1985). ters, 7, 993–997 (2007). DOI: 10.1351/pac198557040603 DOI: 10.1021/nl070026p 176
Copyright of Express Polymer Letters is the property of Budapest University of Technology & Economics andits content may not be copied or emailed to multiple sites or posted to a listserv without the copyright holdersexpress written permission. However, users may print, download, or email articles for individual use.